PHYSICAL REVIEW LETTERS

week ending 6 SEPTEMBER 2013

Microscopic Mechanism for Shear Thickening of Non-Brownian Suspensions Nicolas Fernandez,1 Roman Mani,2 David Rinaldi,3 Dirk Kadau,2 Martin Mosquet,3 He´le`ne Lombois-Burger,3 Juliette Cayer-Barrioz,4 Hans J. Herrmann,2 Nicholas D. Spencer,1 and Lucio Isa1,* 1

Laboratory for Surface Science and Technology, Department of Materials, ETH Zurich, 8093 Zurich, Switzerland Computational Physics for Engineering Materials, Department of Civil, Environmental and Geomatic Engineering, ETH Zurich, 8093 Zurich, Switzerland 3 Lafarge LCR, 38070 Saint Quentin-Fallavier, France 4 Laboratoire de Tribologie et Dynamique des Syste`mes—UMR 5513 CNRS, E´cole Centrale de Lyon, 69130 E´cully, France (Received 9 April 2013; published 3 September 2013) 2

We propose a simple model, supported by contact-dynamics simulations as well as rheology and friction measurements, that links the transition from continuous to discontinuous shear thickening in dense granular pastes to distinct lubrication regimes in the particle contacts. We identify a local Sommerfeld number that determines the transition from Newtonian to shear-thickening flows, and then show that the suspension’s volume fraction and the boundary lubrication friction coefficient control the nature of the shear-thickening transition, both in simulations and experiments. DOI: 10.1103/PhysRevLett.111.108301

PACS numbers: 83.60.Rs, 47.57.E-, 81.40.Pq, 83.80.Hj

Flow nonlinearities attract fundamental interest and have major consequences in a host of practical applications [1,2]. In particular, shear thickening (ST), a viscosity increase from a constant value [Newtonian flow (Nw)] upon increasing shear stress (or rate) at high volume fraction , can lead to large-scale processing problems of dense pastes [3], including cement slurries. Several approaches have been proposed to describe the microscopic origin of shear thickening [4–7]. The most common explanation invokes the formation of ‘‘hydroclusters,’’ which are responsible for the observed continuous viscosity increase [6,8,9] and which have been observed for Brownian suspensions of moderate volume fractions [10,11]. However, this description no longer holds for bigger particles and denser pastes, where contact networks can develop and transmit positive normal stresses [12]. Moreover, the link between hydroclusters and continuous shear thickening (CST) for non-Brownian suspensions is still a matter of debate [13]. Additionally, dense, nonBrownian suspensions can also show sudden viscosity divergence under flow [14–17] with catastrophic effects, such as pumping failures. In contrast to a continuous viscosity increase at any applied rate, defined as CST, the appearance of an upper limit of the shear rate defines discontinuous shear thickening (DST). This CST to DST transition is observed when the volume fraction of the flowing suspension is increased above a critical value, which depends on the system properties, e.g., particle polydispersity or shape, and on the flow geometry [3,18]. An explanation for its microscopic origin is still lacking [19]. Moreover, experiments have demonstrated that the features of the viscosity increase (slope, critical stress) can be controlled by tuning particle surface properties such as roughness [20] and/or by adsorbing polymers [21,22]. These findings suggest that interparticle contacts play a 0031-9007=13=111(10)=108301(5)

crucial role in the macroscopic flow at high volume fractions. A more precise description of these contacts is therefore essential to interpret the rheological behavior. In this Letter, we present a unified theoretical framework, supported by both numerical simulations and experimental data, which describes the three flow regimes of rough, frictional, non-Brownian particle suspensions (Nw, CST, DST) and links the Nw-ST (in terms of shear) and the CST-DST transitions (in terms of volume fraction) to the local friction. Our microscopic particle-contactbased description, as opposed to macroscopic scaling, explains both the occurrence of DST and recovers Bagnold’s analysis [5] for CST, respectively, above and below a critical volume fraction. The lubricated contact between two solid surfaces has been widely studied in the past [23]. It is now commonly accepted that different lubrication regimes occur as a function of a characteristic number, the Sommerfeld number s. For two identical spheres, s ¼ f vRp =N, where f is the fluid viscosity, v is the sliding speed between the two solid surfaces, Rp is the radius of the spheres, and N is the normal load. At high s [‘‘hydrodynamic regime’’ (HD)], a fluid film fully separates the two sliding surfaces and the friction coefficient depends on s. For low s, below a critical value sc , the lubrication film breaks down and contacts between the microscopic asperities on each surface support most of the load. This ‘‘boundary lubrication’’ regime (BL) exhibits friction coefficients that only very weakly depend on s. For intermediate values of s, the system is in a ‘‘mixed regime,’’ where the sharpness of the transition depends on the system properties [e.g., contact roughness, rheology of the fluid; see Fig. 1(a)] [23]. Both experiments and models show that Nw flow is stable below a critical shear rate _ c where the contacts between particles are HD lubricated. On the other hand, a

108301-1

Ó 2013 American Physical Society

PRL 111, 108301 (2013)

PHYSICAL REVIEW LETTERS

FIG. 1 (color online). (a) Schematic Stribeck curve. Evolution of the friction coefficient versus the Sommerfeld number s for a lubricated contact. (b) Apparent viscosity versus the shear rate _ from the numerical simulations. (c) Friction law used in the numerical simulations (black line) and probability distributions of s, PðsÞ, for all contacts at several shear stresses as defined in (b). (d) Frequencies of BL contacts PBL and HD contacts PHD ¼ 1 PBL , as a function of _ for the stresses defined in (b). The simulations data in (b)–(d) have ¼ 0:58, 0 ¼ 0:1, and sc ¼ 5 105 .

particle-contact-dominated flow requires, by definition, that s < sc and it is equivalent to a dense dry granular flow (i.e., no suspending fluid lubrication effects). Dense granular flows follow a quadratic scaling of the normal and shear stress P and with the shear rate _ (Bagnold scaling) through a volume-fraction-dependent factor [5]; this implies that the apparent viscosity rises linearly with _ and that the system shear thickens continuously [see Fig. 1(b)]. This scaling can be expressed in terms of a dimensionless parameqﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ _ p p =P, only depending on ter, the inertial number I ¼ R and for rigid particles with density p [24]. Given the _ p R2p . This Bagnold definition of s, this leads to s / f I 2 = (CST) regime is then possible as long as _ is larger than _ c / f I 2 =sc p R2p , showing the link between _ c and sc when particle contacts dominate. This transition was partially proposed, with macroscopic arguments, by Bagnold [5,25,26]. Nevertheless, our microscopic analysis also accounts for volume-fraction effects. In our model, the existence of two lubrication mechanisms (boundary and hydrodynamic) implies two different jamming volume fractions max , above which flow is not possible. If the system is hydrodynamically lubricated, the jamming volume fraction HD max is the random close packing one RCP , regardless of the boundary friction coefficient 0 [27]. Conversely, when the system is in a boundary-lubricated Bagnold regime, the jamming volume HD fraction BL max decreases with 0 [28,29]. Both max and _ are independent of for non-Brownian particles. It BL max HD BL follows that RCP ¼ max max ð0 Þ. When HD BL max max , the transition from hydrodynamic to boundary-dominated flow is possible and the suspension

week ending 6 SEPTEMBER 2013

exhibits CST, as reported above and predicted by Bagnold. HD When BL max < max , the transition to a Bagnold regime is forbidden, and the shear rate cannot exceed _ c : the system undergoes DST. As a consequence, BL max is the critical volume fraction for DST, and therefore it can be tuned by changing the particle friction coefficient. Both numerical simulations and experiments fully and independently support our model. In concentrated systems, most of the dissipation arises from particles that are in, or close to, contact and not from Stokesian drag [25,30]. This motivates using contact dynamics [31–35] to simulate dense suspensions of hard, spherical, frictional particles using a simplified Stribeck curve (no mixed regime) as friction law [see Fig. 1(c) and Eq. (1)]. Only one dissipative mechanism, either BL or HD, is taken into account in each contact. This constitutes the simplest physical description of a lubricated contact. The boundary lubrication between two rough particles is described using Amontons-Coulomb friction, i.e., the coefficient of friction 0 being independent of the load, the speed and the apparent contact area [23]. In the HD regime, the hydrodynamic interactions between two neighboring particles are long lived and can be described by standard, low-Reynolds-number fluid mechanics with a lubrication hypothesis [36], from which a friction coefficient can be calculated as a function of the Sommerfeld number ¼ 2s lnð5=6sÞ (see the Supplemental Material [37] for a full derivation). The lubrication hypothesis breaks down when the particles are too far apart (i.e., when s is large), and therefore we consider only a range of _ where s of almost all the contacts is smaller than a limit value slim ¼ 101 . The friction law used for the simulations is then 8 < 0 if s < sc ðsÞ ¼ (1) : 2s ln 5 if sc < s < slim : 6s In our contact-dynamics simulations, the normal forces are calculated based on perfect volume exclusion, using zero normal restitution coefficient, and we simulate stresscontrolled () simple shear between moving and fixed rough walls (obtained by randomly glued particles) at a constant volume fraction [38,39]. The rectangular simulation box dimensions are ðLx ; Ly ; Lz Þ ¼ ð25R; 10R; 27RÞ, where Lz is the distance between the two walls and R the radius of the largest particle in the simulations. We use periodic boundary conditions in both x and y directions. The presence of hard confinement mimics experimental conditions. Simulations with Lees-Edwards boundary conditions that are periodic in the three directions show the same qualitative behavior (see the Supplemental Material [37]). The particle radii are uniformly distributed between 0:8R and R to prevent crystallization. When fixing , 0 , R, p , and sc , the physics of the system is characterized pﬃﬃﬃﬃﬃﬃﬃﬃﬃ by a single dimensionless number: ¼ p R=f . can be understood as the ratio between the microscopic time scale of the lubricating fluid f = and of the granular

108301-2

week ending

PHYSICAL REVIEW LETTERS 6 SEPTEMBER 2013 PRL 111, 108301 (2013) qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ CST-DST transition occurs when is increased above medium R p = [24]. Increasing the shear stress quadratiBL max ð0 ¼ 0:3Þ compatible with Ref. [28]. cally is equivalent to decreasing f linearly. In our simulaIn brief, the numerical simulations confirm that our tions, we vary f and keep fixed. After the system has theoretical framework sets the sufficient conditions to reached its steady state with a linear velocity profile (no shear explain Nw-ST and CST-DST transitions. bands), we measure the time-averaged velocity of the movOur model is also independently supported by experiing wall hvwall i; thus, _ ¼ hvwall i=Lz and the apparent visments where the link between local friction and macro_ The quantities , _ cosity of the suspension is given by =. scopic rheology is established using quartz surfaces. We , and are measured in units of f =p R2 , 2f =p R2 , and first show experimentally that the volume fraction of the CST-DST transition is indeed BL f (see the Supplemental Material [37] for details). max and then that it can be tuned by modifying 0 . This is demonstrated by using The simulations [see Figs. 1(b) and 2] reproduce a four different comb polymers, i.e., poly(methacrylic acid) transition between a Newtonian regime at low shear rates (PMAA) grafted with poly(ethylene glycol) (PEG) side (independent of 0 and dominated by HD-lubricated chains, which are dissolved in a CaðOHÞ2 -saturated aque_ for which contacts) to a ST regime with increasing , ous buffer solution with 20 mmol=L K2 SO4 . The copolyboundary-lubricated contacts are dominating. In the mers were synthesized by radical polymerization in water absence of hydrodynamics in the friction law, such a according to Refs. [40,41]. Their specifications, obtained transition is lost (see the Supplemental Material [37]). from aqueous gel permeation chromatography, are Indeed, in Fig. 1(c) for increasing applied stress, the dis(backbone size in kDa, number of carboxylic acids per tributions of s in all the particle contacts shift toward the side chain, and side chain size in kDa) polymer A, PMAA BL regime in the Stribeck curve. In our simulations, the (4.3)-g(4)-PEG(2); polymer B, PMAA(3.4)-g(2.3)-PEG(2); system shear thickens when at least 20% of the contacts polymer C, PMAA(4.3)-g(4)-PEG(0.5); and polymer D, are below sc . In Fig. 1(d), the percentage of contacts in BL PMAA(5)-g(1.5)-PEG(2). Once in the buffer solution, these and HD regimes is plotted against _ for the stresses defined comb polymers are readily adsorbed onto a negatively in Fig. 1(b). For low 0 , this ST regime is continuous and charged surface, such as quartz, by calcium-ion bridging, _ Here, the viscosity fits with a Bagnoldian scaling ( / ). and create a stable and highly solvated PEG coating on the increases with 0 , as in a dry granular medium [24]. This solid surface [42] that is known to modify the BL coefficient scenario changes as 0 goes beyond a critical value, here of friction [43]. The conclusions of the experiments are not 0.35 for ¼ 0:58 (Fig. 2). Then, the system can no longer dependent on the choice of system, which is a model be sheared above a critical shear rate for any shear stress: material for industrial applications (e.g., cement slurry), the system shear thickens discontinuously. for which the friction coefficient can be easily tuned. The transition from CST to DST does not only occur The rheological analysis was performed on suspensions when increasing 0 but also when increasing : the system of ground quartz (Silbelco France C400, D50 ¼ 12 m) experiences CST at ¼ 0:58 and 0 ¼ 0:3 but experienwith between 0.47 and 0.57 in the alkali polymer soluces DST for ¼ 0:59 and the same 0 (see Fig. 2). tions (see the Supplemental Material [37] for details). We Moreover, as predicted in our theoretical model, the initially measured BL via compressive rheology by highmax

FIG. 2 (color online). Apparent viscosity versus _ for different 0 and sc ¼ 5 105 in simulations. In the Newtonian regime, the viscosity does not depend on 0 but on . At ¼ 0:58, for 0 0:3, the system experiences CST, where the viscosity depends on the friction coefficient. For 0 0:35, the system _ Data points for ¼ 0:59 show DST jams at sufficiently large . for 0 ¼ 0:3. Inset: Zoom of the transition zone.

speed centrifugation (acceleration 2000g) of a fairly low concentration suspension ( ¼ 0:47) in a 10 mL measuring flask and calculated the average sediment volume fraction for the various polymers. During sedimentation at high speed, particles come into contact and jam, producing a looser sediment compared to frictionless objects. After 20 min of centrifugation, no further evolution is observed BL and we measured BL max ðAÞ ¼ 0:578, max ðBÞ ¼ 0:560, BL BL max ðCÞ ¼ 0:555, and max ðDÞ ¼ 0:545 [see Fig. 3(a)]. The CST-DST transition was then measured by shear rheometry in a helicoidal paddle geometry (Anton Paar 301 rheometer; see Ref. [21], Fig. 4, for a geometry description) with a descending logarithmic stress ramp after preshear (from 700 to 0.01 Pa in 100 s). The viscosity curves are divided into two main parts: at low shear rate, the fluid shows a Newtonian behavior with a viscosity that depends on volume fraction [44] [Fig. 3(b)] but not on the polymer coating [Fig. 3(c)]. For high shear rates, the fluid shear thickens. At moderate volume fractions, the system undergoes CST with / _ 2 (Bagnoldian regime) as observed by Ref. [45], while for the higher volume fractions in our

108301-3

PRL 111, 108301 (2013)

PHYSICAL REVIEW LETTERS

experiments, the abruptness of ST increases quickly at a critical [see Fig. 3(b) for polymer A]. Above this threshold, the suspensions display DST. In order to quantify this critical volume fraction, the flow curves for the various in the ST regime are fitted by an Oswald–de Waele power law: / _ n . In Fig. 3(d), we show that nðÞ diverges at the polymer-dependent BL max that we measured independently by centrifugation, as predicted by our model. Moreover, the data from the different polymer coatings collapse onto a single master curve as a function of a BL reduced volume fraction ðBL max Þ=max that does not depend on surface properties. A similar collapse was observed for particles of different shapes [46]. To complete our analysis, we measured the BL friction coefficients 0 between a polished rose quartz stone surface (Cristaux Suisses, Switzerland) and a 2 mm diameter borosilicate sphere (Sigma-Aldrich, USA) coated with the four different polymers, using a nanotribometer (CSM Instruments, Switzerland). The contact was immersed into a drop of polymer solution. The experiments were realized in an N2 atmosphere at sliding velocities between 105 and 103 m=s (see the Supplemental Material [37] for a protocol). The measured values of 0 reported in Fig. 4 are speed-independent, as expected in the BL regime. The differences in the friction for the different

FIG. 3 (color online). (a) Sediment heights for the different polymers after centrifugation. (b) Viscosity versus shear rate with adsorbed polymer A for various of quartz microparticle suspensions. (c) Viscosity versus shear rate for the four adsorbed polymers at analogous [ðAÞ ¼ 0:537, ðBÞ ¼ 0:537, ðCÞ ¼ 0:538, and ðDÞ ¼ 0:535]. (d) Oswald–de Waele exponent n versus the reduced volume fraction [same symbols as in (c)]. Inset: Same data as in the log-log plot. The solid line is a power-law fit for (n 1) versus reduced volume fraction.

week ending 6 SEPTEMBER 2013

polymers have been previously ascribed to a variation of the PEG unit density on the surfaces [47], stemming from an equilibrium between entropic side chain repulsion and electrostatic attraction between the backbone and the surface (through calcium bridging). Finally, Fig. 4 shows the direct correlation between the BL coefficients of friction and the measured maximum volume fraction BL max that separates CST and DST, as included in our model. BL max is a decreasing function of the particle friction coefficient in the boundary regime, as predicted by simulations [28,29]. Using a simple theoretical framework, independently backed up by simulations and experiments, we have identified the microscopic origin of both continuous and discontinuous shear thickening of dense non-Brownian suspensions as the consequence of the transition from hydrodynamically lubricated to boundary-lubricated contacts. The central role played by friction introduces the local Sommerfeld number as the controlling parameter, as demonstrated by our numerical simulations. The presence of two distinct lubrication regimes as a function of the Sommerfeld number is therefore at the origin of the Nw-ST transition. In particular, the friction coefficient in the boundary regime, which we tuned experimentally by polymer adsorption on the particle surface, governs the nature of the ST transition. Distinct lubrication regimes imply that the jamming volume fractions in the viscous regime HD max and in the Bagnoldian regime BL max are not the same in general, given that only the latter depends on the friction BL coefficient. Therefore, CST is found when HD max max , while the suspension exhibits DST when the transition to BL the inertial regime is impossible because HD max > max . Thus, in the absence of transient migration effects [45], the local volume fraction and friction coefficient determine the stable microscopic flow mechanism, which is either CST or DST [45,48,49]. Moreover, our model does not require any confinement at the boundaries, but only that locally > BL max . This condition is fulfilled by preventing particle migration out of the shear zone, either by confinement during

FIG. 4 (color online). BL max as a function of the coefficient of friction in boundary regime 0 for the four polymers (same symbols as in Fig. 3). The CST and DST regions are highlighted in the graph.

108301-4

PRL 111, 108301 (2013)

PHYSICAL REVIEW LETTERS

steady-state shear [18] or by keeping the shear duration short enough [50]. The generality and consistency of our data and of the proposed model set a global framework in which the tribological (friction) and rheological properties of dense noncolloidal systems are intimately connected. This concept is expected to have an impact on a host of practical applications and relates fundamental issues such as flow localization [51] and the solid-liquid-solid transition of granular pastes [14]. The authors thank Fabrice Toussaint for scientific discussions during preliminary work and Ce´dric Juge, Abdelaziz Labyad, and Serge Ghilardi for technical support. The authors acknowledge financial support by Lafarge LCR. Furthermore, this work was supported by the FP7-319968 Grant of the European Research Council, the Ambizione Grant No. PZ00P2_142532/1 of the Swiss National Science Foundation, and the HE 2732/11-1 Grant of the German Research Foundation.

*Corresponding author. [email protected] [1] R. Larson, The Structure and Rheology of Complex Fluids (Oxford University, New York, 1999). [2] P. Coussot and C. Ancey, Rhe´ophysique des Paˆtes et des Suspensions (EDP Sciences, Les Ulis, 1999). [3] H. Barnes, J. Rheol. 33, 329 (1989). [4] E. Andrade and J. Fox, Proc. Phys. Soc. London Sect. B 62, 483 (1949). [5] R. A. Bagnold, Proc. R. Soc. A 225, 49 (1954). [6] J. F. Brady and G. Bossis, J. Fluid Mech. 155, 105 (1985). [7] R. Hoffman, Trans. Soc. Rheol. 16, 155 (1972). [8] W. Boersma, J. Laven, and H. N. Stein, AIChE J. 36, 321 (1990). [9] N. J. Wagner and J. F. Brady, Phys. Today 62, No. 10, 27 (2009). [10] J. Bergenholtz, J. F. Brady, and M. Vicic, J. Fluid Mech. 456, 239 (2002). [11] X. Cheng, J. H. McCoy, J. N. Israelachvili, and I. Cohen, Science 333, 1276 (2011). [12] M. E. Cates, J. P. Wittmer, J. P. Bouchaud, and P. Claudin, Phys. Rev. Lett. 81, 1841 (1998). [13] J. Morris, Rheol. Acta 48, 909 (2009). [14] A. Fall, N. Huang, F. Bertrand, G. Ovarlez, and D. Bonn, Phys. Rev. Lett. 100, 018301 (2008). [15] L. Isa, R. Besseling, A. Morozov, and W. Poon, Phys. Rev. Lett. 102, 058302 (2009). [16] E. Brown and H. Jaeger, Phys. Rev. Lett. 103, 086001 (2009). [17] E. Brown, N. A. Forman, C. S. Orellana, H. Zhang, B. W. Maynor, D. E. Betts, J. M. DeSimone, and H. M. Jaeger, Nat. Mater. 9, 220 (2010). [18] E. Brown and H. Jaeger, arXiv:1010.4921. [19] P. Coussot and N. J. Wagner, Rheol. Acta 48, 827 (2009). [20] D. Lootens, H. Van Damme, Y. He´mar, and P. Hebraud, Phys. Rev. Lett. 95, 268302 (2005). [21] F. Toussaint, C. Roy, and P. H. Je´ze´quel, Rheol. Acta 48, 883 (2009). [22] H. Lombois-Burger, P. Colombet, J. Halary, and H. Van Damme, Cem. Concr. Res. 38, 1306 (2008).

week ending 6 SEPTEMBER 2013

[23] G. W. Stachowiak and A. W. Batchelor, Engineering Tribology (Butterworth-Heinemann, Oxford, 2005). [24] Y. Forterre and O. Pouliquen, Annu. Rev. Fluid Mech. 40, 1 (2008). [25] M. Trulsson, B. Andreotti, and P. Claudin, Phys. Rev. Lett. 109, 118305 (2012). [26] F. Boyer, E´. Guazzelli, and O. Pouliquen, Phys. Rev. Lett. 107, 188301 (2011). [27] N. Roussel, A. Lemaıˆtre, R. Flatt, and P. Coussot, Cem. Concr. Res. 40, 77 (2010). [28] L. E. Silbert, Soft Matter 6, 2918 (2010). [29] M. P. Ciamarra, R. Pastore, M. Nicodemi, and A. Coniglio, Phys. Rev. E 84, 041308 (2011). [30] N. A. Frankel and A. Acrivos, Chem. Eng. Sci. 22, 847 (1967). [31] J. J. Moreau, Eur. J. Mech. A. Solids 13, 93 (1994). [32] M. Jean and J. J. Moreau, Proceedings of Contact Mechanics International Symposium (Presses Polytechniques et Universitaires Romandes, Lausanne, 1992), p. 31. [33] L. Brendel, T. Unger, and D. E. Wolf, The Physics of Granular Media (Wiley-VCH, Weinheim, 2004). [34] R. Mani, D. Kadau, D. Or, and H. J. Herrmann, Phys. Rev. Lett. 109, 248001 (2012). [35] D. Kadau, J. Andrade, Jr., and H. Herrmann, Eur. Phys. J. E 30, 275 (2009). [36] D. Barthes-Biesel, Microhydrodynamics and Complex Fluids (CRC Press, Boca Raton, FL, 2012). [37] See Supplemental Material at http://link.aps.org/ supplemental/10.1103/PhysRevLett.111.108301 for additional details on the numerical simulations (derivation of the friction law, parameter variation, role of lubricating fluid and confining walls) and experiments (rheology and friction measurements). [38] M. La¨tzel, S. Luding, H. J. Herrmann, D. W. Howell, and R. P. Behringer, Eur. Phys. J. E 11, 325 (2003). [39] A. Pea, P. Lind, S. McNamara, and H. Herrmann, Acta Mech. 205, 171 (2009). [40] D. Rinaldi, T. Hamaide, C. Graillat, F. D’Agosto, R. Spitz, S. Georges, M. Mosquet, and P. Maitrasse, J. Polym. Sci. A 47, 3045 (2009). [41] J. A. Jones, N. Novo, K. Flagler, C. D. Pagnucco, S. Carew, C. Cheong, X. Z. Kong, N. A. D. Burke, and H. D. H. Sto¨ver, J. Polym. Sci. A 43, 6095 (2005). [42] R. J. Flatt, I. Schober, E. Raphael, C. Plassard, and E. Lesniewska, Langmuir 25, 845 (2009). [43] S. Lee and N. D. Spencer, Science 319, 575 (2008). [44] I. M. Krieger and T. J. Dougherty, Trans. Soc. Rheol. 3, 137 (1959). [45] A. Fall, A. Lemaıˆtre, F. Bertrand, D. Bonn, and G. Ovarlez, Phys. Rev. Lett. 105, 268303 (2010). [46] E. Brown, H. Zhang, N. A. Forman, B. W. Maynor, D. E. Betts, J. M. DeSimone, and H. M. Jaeger, Phys. Rev. E 84, 031408 (2011). [47] S. S. Perry, X. Yan, F. T. Limpoco, S. Lee, M. Mu¨ller, and N. D. Spencer, ACS Appl. Mater. Interfaces 1, 1224 (2009). [48] A. Fall, Ph.D. thesis, Universite´ Paris VII, 2008. [49] A. Fall, F. Bertrand, G. Ovarlez, and D. Bonn, J. Rheol. 56, 575 (2012). [50] S. R. Waitukaitis and H. M. Jaeger, Nature (London) 487, 205 (2012). [51] N. Huang, G. Ovarlez, F. Bertrand, S. Rodts, P. Coussot, and D. Bonn, Phys. Rev. Lett. 94, 028301 (2005).

108301-5